UNIVERSITÀ DEGLI STUDI DI PARMA
FACOLTÀ DI FARMACIA
DOTTORATO DI RICERCA IN BIOFARMACEUTICA-FARMACOCINETICA
MICROPARTICULATE DRUG DELIVERY SYSTEMS BASED ON HYDROPHILIC POLYMERS OBTAINED
WITH A SUPERCRITICAL CO2
Chiar.mo Prof. Ruggero Bettini Coordinatore:
Chiar.mo Prof. Paolo Colombo
Tesi di Dottorato:
XX CICLO 2005-2007
To my family and Nicola
This thesis includes the paper listed below:
1. I. Pasquali, R. Bettini, F. Giordano, Solid-State Chemistry and Particle Engineering with Supercritical Fluids in Pharmaceutics, Eur. J. Pharm. Sci., 27, 299-310 (2006).
2. I. Pasquali, R. Bettini, F. Giordano, Supercritical fluid technologies: an innovative approach for the manipulation of the solid-state of pharmaceuticals, Adv. Drug Del. Rev. In press, doi: 10.1016/j.addr.2007.08.030.
3. I. Pasquali, L. Comi, F. Pucciarelli, R. Bettini, Swelling, melting point reduction and solubility of PEG 1500 in supercritical CO2, Int. J. Pharm, in press, doi:10.1016/j.ijpharm.2007.12.048.
4. I. Pasquali, J.-M. Andanson, S. G. Kazarian, R. Bettini, Measurement of CO2 sorption and PEG 1500 swelling by ATR-IR spectroscopy, J. Supercrit. Fluids, accepted.
5. I. Pasquali, J.-M Andanson, S. G. Kazarian, R. Bettini, Solubility of diazepam in PEG 1500 under supercritical CO2 by FT-IR spectroscopy, in preparation for Int. J. Pharm.
6. I.Pasquali, R. Bettini “Are pharmaceutics really going supercritical?” Invited review for Int. J. Pharm., in preparation
7. I. Pasquali, L. Pezzini, R. Menabeni, R. Bettini, Diazepam microparticles with improved biopharmaceutical properties obtained with PGSS method, in preparation for Eur. J. Pharm. Biopharm.
1. Introduction 1
1.1 Supercritical fluids properties 3
1.2 Processes using supercritical fluids 8
1.2.1 Processing using supercritical fluids as solvent 8 RESS (Rapid Expansion Supercritica Solution) 8 RESOLV (Rapid Expansion of a Supercritical solution into a Liquid Solvent) 11
1.2.2 Processing using supercritical fluids as antisolvent 11
GAS (Gaseous Anti Solvent) 14
PCA (Particles by Compressed Antisolvent), SAS (Supercritical Antisolvent) ASES (Aerosol Solvent Extraction System) 15 SEDS (Solution Enhanced Dispersion by Supercritical Fluids) 15
1.2.3 CO2-assisted spray-drying 17
CAN-BD (Carbon dioxide Assisted Nebulization with a Bubble Dryer®) 17 SAA (Supercritical Fluid-Assisted Atomization) 18 1.2.4 Precipitation from gas saturated solutions 19
PGSS (Particle formation from Gas-Saturated Solution ) 19 DELOS (Depressurization of an Expanded Liquid Organic Solution) 20 CPSP (Continuous Powder Coating Spraying Process) 21
1.3 Phase behaviour 22
1.3.1 Unitary system (one component) 23
1.3.2 Bynary system (two components) 23
1.3.3 Ternary system (three components) 30
1.4 Polymer processing using SC-CO2 31
1.4.1 Polymer-CO2 phase behaviour (Liquid-Liquid phase behaviour) 31
1.4.2 Pressure Induced Phase Separation (PIPS) 32
1.4.3 Solubility of CO2 in polymers and viceversa 34
1.4.4 Polymer plasticization 36
1.5 Polyethylene glycols (PEGs) 38
1.6 Diazepam 41
3 Matherials and Methods 44
3.1 Materials 44
3.2 Methods 44
3.2.1 HPLC assay 44
PEG 1500 44
Linearity 45 Precision or Relative Standard Deviation (RSD) 45
Limit of detection 46
Limit of quantitation 46
Number of theoretical Plates (n) 46
Tailing factor 47
3.2.2 Measurament of the density of PEG 1500 and CO2 48
3.2.3 High-pressure view cell 48
Melting point under SC-CO2 48
Polymer swelling under SC-CO2 49
3.2.4 PEG 1500 solubility in SC-CO2 49
3.2.5 CO2 solubility in PEG 1500 51
3.2.6 ATR-FTIR apparatus 52
Measurement of CO2 sorption and PEG 1500 swelling 54 Solubility of diazepam in PEG 1500 under SC-CO2 54
3.2.7 Solubility of diazepam in SC-CO2 55
3.2.8 Preparation of PEG microparticles loaded with diazepam 57
3.2.9 Vibration mill 58
3.2.10 Drug content uniformity in the microparticles 58
3.2.11 Powder x-ray diffraction (PXRD) 58
3.2.12 Differential scanning calorimetry (DSC) 60
3.2.13 Scanning electron microscopy (SEM) 60
3.2.14 Laser diffraction particle size analysis 61
3.2.15 Aerodynamic assessment using Andersen Cascade Impactor (ACI) 61
Silicon cast 66
3.2.17 Dissolution studies 67
4 Results and Discussion 69
4.1 HPLC validation 69
4.1.1 PEG 1500 69
4.1.2 Diazepam 70
4.2 PEG 1500 and 4000 characterization 71
4.3 Diazepam characterization 75
4.4 PEG/CO2binary system 80
4.4.1 Melting point under supercritical CO2 80
4.4.2 Polymer swelling under supercritical CO2 by using the high-pressure view cell 82 4.4.3 Solubility of PEG 1500 in supercritical CO2 83 4.4.4 CO2 solubility in PEG 1500 by gravimetric method 88 4.4.5 Measurement of CO2 sorption and PEG 1500 swelling by
ATR-FTIR spectroscopy 89
Quantitative analysis 92
PEG 1500 swelling and CO2solubility 95
4.4.6 Discussion on the solubility and swelling data 97
4.5 PEG 1500/diazepam/CO2system 101
4.5.1 Quantitative analysis 101
4.5.2 Solubility data 104
4.6 Diazepam/CO2system 108
4.6.1 Quantitative analysis 108
4.6.2 Solubility data 108
4.7 Production of the PEG 1500 and 4000 microparticles loaded with diazepam 109
4.7.1 Yield of the process 110
4.7.2 Drug content of the microparticles 111
4.7.3 Particle size distributions and morphology study 112
4.7.6 Crystallinity of the microparticles 124
4.7.7 Dissolution study 126
5. Conclusions 128
The founders of “Pharmaceutics” brought the science of physical chemistry to drug delivery, recognizing “Pharmaceutics” as the science of rationale dosage form development.
The design and the production of effective, stable, uniform and safe dosage forms that contain exact quantities and specific qualities of active pharmaceutical ingredients (APIs) is the primary mission of the pharmaceutical industry. The quality of a product is strongly related to and influenced by its design in research and development.
In the case of the solid dosage form a great attention has been paid, in recent years, on particle engineering defined as the discipline enabling the scientist to design solid dosage forms tailored to possess optimal physico-chemical characteristics (Pasquali et al., 2006).
Specific characteristics of particles (size, shape, surface, crystal structure and morphology) are among the important factors to control technological and biopharmaceutical properties of drug products. In general, morphology (crystal habit) can influence the physical and chemical stability of solid dosage forms, a narrow size distribution is important to obtain content uniformity, while sphericity allows good flowability and tablettability.
Furthermore, micronisation increases the surface area with a consequent increase of dissolution rate and bioavailability of the drug, thus promoting the formulation of active principle ingredients which may be insoluble or slightly soluble in aqueous media. Finally, the increase of bioavailability maximizes the efficiency of the drug and hence minimizes the required dosage.
Technological and biopharmaceutical characteristics can also be improved by co- formulation of the API with polymers. Co-formulations are used to increase (fast-release) or decrease (sustained release) the dissolution rate of the drug, for taste-masking, where a drug is co-formulated to remove or disguise an unpleasant taste, and in general to improve technological characteristics such as: sphericity, flowability, tabletability etc.
Formulation of drug delivery systems implies the challenge of producing particles with optimal physico-chemical characteristics, especially in the case of an administration by parenteral or inhalation route. For inhalation route, particles with a size less then 5 μm, narrow particle size distribution, appropriate aerodynamic size, shape and apparent density are required. Whilst is crucial to control the aerodynamic particle size, it is also important to control the surface properties as micronized tend to be highly charged leading to agglomeration. Furthermore, some techniques used to reduce particle sizes (milling, spray-
drying) damage the crystal structure of the drug leading to total or partial amorphisation, which leads to the physical instability of the drug.
Meanwhile, there is a continuous effort to develop processes pollution-free, with low environmental impact. Numerous pharmaceutical processes use volatile organic compound (VOC) as medium for preparation of drug delivery systems, but VOCs emission limit are being reduced in many industrialised countries, for example the European Union legislation came into force in 2000 (Hay et al., 2002). Furthermore, the “green”
alternatives has become very important, especially in case of pharmaceutical industries, because the regulatory requirements are more and more restrictive for the residual contents of volatile organic compounds in the API and in the final products. A “green” solvent, alternative to traditional solvents, may lead both to a technical and commercial benefits.
A relatively recent approach for obtaining pharmaceutical microparticles with desired physico-chemical characteristics is represented by technologies based on the supercritical fluids (SCF). By proper adjustment of the operating conditions as well as physical and chemical parameters, (pressure, temperature, drug concentration, flow and nature of supercritical fluid and organic solvent) materials with desired biopharmaceutical and technological characteristics can be generated. Advantages in the use of supercritical fluids technology are the high versatility, the flexibility in offering alternative processing approaches, the possibility to avoid or minimize the use of organic solvents and to reach peculiar process conditions (i.e., change in the pressure and in the rate of solvent evaporation) difficult to obtain with traditional processes (Pasquali et al., in press-b). In fact, the most discernible process parameters that differentiate the SCF technologies from the conventional ones are the high compressibility and diffusivity of the supercritical fluid, the possibility of fine tuning pressure and solvent evaporation rate.
Great attention is given to the SCFs also in the field of polymer processing (Nalawade et al., 2006a). Most of the beneficial effects of SCF in the polymers processing are due to the possible weak interaction of CO2 with the macromolecular chains of the polymer. As demonstrated by some authors (Kazarian et al., 1996, Nalawade et al., 2006b, Pasquali et al., in press-a), CO2 is a weak Lewis acid that may interact with the basic sites in the polymer leading to the absorbtion of significant amount of CO2. The absorption of the gas results in an increase of the inter-chain distances as well as of the degree of chains- segmental mobility causing a polymer plasticization and a decrease of the polymer viscosity. The property of CO2 to reduce the glass transition temperature and viscosity of
the polymer would be beneficial for enhancing in the processing of composite materials during mixing, homogenization, coating, extrusion and foaming.
Polymer plasticization can be also induced thermally or by means of organic solvents.
Major drawbacks of these approaches are the difficulty to process heat-sensitive materials and the possible presence of residues solvent in the final product. By using the SCF, there is no residual solvent in the material produced, in fact, being a gas at ambient condition, it can easily be removed from the final product.
The application of the SFC technology in the control of physico-chemical properties of drug particles (Pasquali et al., 2006, Pasquali et al., in press-b) and the production of controlled-release drug formulations seems to have at the moment a big development, as reflected by the large number of patents granted in this area.
Despite the numerous advantages in the use of SCF, it must be stated that these techniques are not going to replace existing and well-established techniques (solvent coating, granulation, spray-drying, etc.); but more likely they are going to support them.
One of the major drawbacks of the SCF techniques presently represented by the high cost of the equipments. This can be mainly ascribed to the fact that the field is still young and the SCF technologies are not yet widespread.
1.1. Supercritical fluids properties
In 1822, Cagniard de la Tour first put into evidence the existence of a supercritical phase by observing the disappearance of two distinct gas and liquid phases into one visually homogeneous phase by increasing the temperature of a material in a closed glass container (Cagniard de LaTour, 1822).
The first report that describes a process using the supercritical fluid as a medium for obtaining solid materials was published by Hannay and Hogarth: “ We have then, the phenomenon of a solid with no measurable gaseous pressure, dissolving in a gas. When the solid is precipitated by suddenly reducing the pressure, it is crystalline, and may be brought down as snow in the gas, or on the glass as a frost, but it is always easily redissolved by the gas on increasing the pressure” (Hannay and Hogarth, 1879).
A supercritical fluid can be defined as a dense non-condensable fluid.
A fluid reaches the supercritical status when its temperature and pressure exceed the relevant critical temperature and pressure.
Figure 1: Images of the CO2 at different pressure and temperature values (http://www.galenotech.org/tecniche_est.htm)
As it can be observed in Figure 1, below the critical point a liquid and a gas phase are separated by a meniscus; with an increase in temperature or pressure the meniscus begins to disappear. Further increase of temperature causes the gas and liquid densities to become similar. The meniscus is less easily observed but still evident. Once the critical temperature and pressure have been reached the two distinct phases (liquid and gas) are no longer visible. The macroscopic appearance of the SCF is a homogeneous and opalescent system without phase separation (single phase) because, at this point, the density of the gas and liquid are identical. Nevertheless, a SCF does not show a specific aggregation state; in fact its physico-chemical properties are intermediate between those of liquid and gas (Table 1).
Table 1. Physico-chemical characteristics of a substance as gas, liquid and SCF.
* standard condition (1 atm, 20 °C) **at critical pressure and temperature
Like a gas the SCF shows a lower viscosity and higher diffusivity relative to the liquid.
These properties facilitate mass transfer and all related phenomena, so SCFs can diffuse and impregnate matrices like a gas. Like a liquid, the SCF shows a density value appreciable for the solvation power. Most importantly, the SCF is dense but highly
Physical state Density (g / ml)
Viscosity ( g/cm⋅s)
Diffusivity (cm2/ s)
Gas* 10-3 10-4 10-1
Liquid 1 10-2 10-6
SCF** 0.2 –0.8 10-4 10-3
compressible, thus, any change of pressure alters its density and consequently the solvent power (Brunner, 1994). The greatest change of the solvent density is attained in the vicinity of the solvent’s critical point, where the solvent compressibility is large, and small changes in pressure yield a large change in density (Figure 2).
Figure 2. Carbon dioxide density-pressure phase diagram
At the microscopic level, the opalescence observed at the critical point can be interpreted considering the fluctuations of the local density with a correlation length of the same order of magnitude than that of the visible light. The inhomogenity is the most fundamental concept which characterizes the supercritical status, and the density fluctuations is a measure of the inhomogenity in the distribution of the molecules. It has been reported that there is likely a local organization of molecules inside the supercritical region with areas of local densities for both the gas and liquid (Nishikawa and Morita, 2000). This organization is dynamic and these fluctuations of density allow to explain the increase of the fluid compressibility. Inside the schematic phase diagram of CO2 near the critical point, (Figure 3) it is possible to identify a ridge that separates the more liquid-like and more gas-like regions in the supercritical region.
Figure 3. Schematic phase diagram of CO2
The ridge corresponds to a maximum or minimum of various physical quantities of SCFs, which are related to the second derivates of the Gibbs free energy, such as isothermal compressibility, thermal conductivity, and partial molar volumes (Koga et al., 2006).
Although these unique and complementary physical characteristics allow the development of efficient and versatile processes, it should be underscored that the SCF can not be considered as the universal “super-solvent”.
The peculiar characteristics of SCFs lead to a rapidly grown of the field, and of consequence, to important industrial applications (Perrut, 2000, Perrut, 2003). Except for processes applied in the petrochemical industry, supercritical fluids applications are mainly focusing on extraction/fractionation from solid materials for food products (coffee and tea), food ingredients (hops, aromas, coloring agents, vitamins, and unsatured fatty acids) and nutraceuticals/phytopharmaceuticals (Jung and Perrut, 2001, King and Bott, 1993, Perrut and Reverchôn, 2000, Perrut and Subra, 1998, Poliakoff et al., 1999, Rizvi, 1994). At present, supercritical fluids techniques are still expanding and new applications are being investigated. Some of them are listed below:
• Ceramics manufacture: preparation of a new generation of inorganic cross-flow membranes (Sarrade et al., 2003);
• Reactions: synthesis of complex organic molecules (Prajapati and Gohain, 2004);
• Preparative Scale Supercritical Fluid Chromatography: fractionation of very similar compounds, especially lipids;
• Preparation of foams (Alavi et al., 2003a, Alavi et al., 2003b) and aerogels (Fricke and Tillotson, 1997, Gross et al., 1998 ). Various SF-processed nano-systems or nano- structured materials for applications mainly in the micro-electronic industry; (Perrut, 2000)
• Polymer processing: impregnation, extraction of residues (stripping), morphological modifications (foams, particles, and fibers) and particle coating.
Among the new applications of SCFs, particle engineering of pharmaceutical materials seems to be at the moment the area with the major development.
All gases can be a SCF above specific sets of critical conditions (P,T), but it should be born in mind also that, for many cases, the transition to the supercritical state occurs at high temperatures not compatible with pharmaceutical compounds (e.g., SC water, Table 2).
Table 2: Critical parameters of selected compounds
Tc (°C) Pc (MPa)
H2O 374 22
Xe 16.6 5.9
SF6 45.5 3.8
N2O 36.5 4.1
C2H4 9.1 5.1
CHF3 25.9 4.7
CO2 31.3 7.4
The critical P, T values increase with the molecular weight or intermolecular hydrogen bonding or polarity (Vasukumar and Bansal, 2003). Not only the mild processing conditions, but also safety and affordable economics are valid criteria to choose the supercritical fluid. For example, Xenon and SF6 (when sufficiently purified), have low critical values, but they are still too expensive for commercial use. Gases as N2O or ethane have low critical values, but can generate explosive mixtures and are therefore unsafe to handle. Some authors (Hillmann and Bächmann, 1995, Nakatani et al., 1989, Sako et al., 1989) used as SCF trifluoromethane (CHF3) which is chemically inert, non-flammable, has
low toxicity and low critical temperature and pressure. Furthermore, CHF3 has a strong permanent dipole moment (1.56 D) thus it can solubilize pharmaceutical compounds.
However, more than 98 % of applications have been developed using carbon dioxide as SCF because of its low critical temperature (31,18 °C) and pressure (7.4 MPa), inexpensiveness, non–flammability, non-toxicity, recyclability and environmental benignity.
1.2. Processes using supercritical fluids
There are several methods based on the supercritical fluids for particles production, which can be divided into four groups.
i) Processes using supercritical fluids as solvent. The rapid expansion of a supercritical solution (RESS) is the process that exemplifies this first group. The supercritical fluid is used as crystallization solvent; in fact, with RESS the solute is first dissolved in a supercritical fluid, then the solution is rapidly expanded by sudden decompression, typically by passing through an orifice at lower pressure.
ii) Processes using supercritical fluids as antisolvent. In this case, the supercritical fluid (antisolvent) comes in contact with the solute dissolved in a suitable organic solvent. The crystal formation is due to the sharp decrease of the solvent power of the organic phase.
iii) Processes using supercritical fluids to assist the spray-drying thechnique. These techniques are close to the classic micronization by spray-drying, where the SCFs is used to assist the nebulization of the solution of the compound to be process.
iiii) Processes using supercritical fluids to precipitate molten material from gas saturated solution. The supercritical fluid is dissolved into a solution of a solute or into a melted material. Then, a rapid depressurization of the mixture, that occurs through a nozzle causing the particles formation.
1.2.1 Processes using supercritical fluids as solvent RESS (Rapid Expansion Supercritical Solution)
Nearly a century later the discovery of Hannay and Hogarth, Krukonis first applied the concept of producing fine particles with a narrow size distribution using a SCF (Krukonis, 1984). This technique was called rapid expansion of a supercritical solution (RESS). A
typical RESS process is carried out with an apparatus consisting of a pre-heater, a solubilization vessel, and a precipitator (Figure 4).
Figure 4. Schematic representation of RESS
The heated gas is pressurized and pumped into the solubilization unit (extractor), containing the solute. The supercritical fluid dissolves the solute; then the solution is rapidly expanded (decompressed) by passing through a heated nozzle at supersonic speed.
During the rapid expansion of the supercritical solution, both density and solvent power decrease dramatically leading to a solute supersaturation. The solution reaches almost instantaneously, a highly homogeneous supersaturation with a degree of supersaturation often much higher than that achieved by thermal methods. The combination of large, rapid and uniform supersaturation is the major advantage of RESS and leads to the production of small particles with uniform size (Phillips and Stella, 1993)
The parameters that influence this process can be divided into pre- and post-expansion conditions. The pre-expansion conditions are temperature and pressure of the vessel. These operative parameters influence the kinetics of the crystallization process changing the density of the SCF and, consequently, the pre-expansion concentration. This last depends also on the supercritical fluid, the nature of the solute (crystalline or amorphous, composite or pure), and possible addition of a cosolvent. The higher the pre-expansion concentration, the narrower the particle size range will be (Phillips and Stella, 1993)
The post-expansion conditions depend on the nozzle temperature, geometry and size, distance and angle of impact against the surface of the jet stream (Kayrak et al., 2003) (Figure 5).
Figure 5. Schematic draw of the nozzle in the RESS process (Kayrak et al., 2003)
The nozzle can be maintained at a suitable pre-expansion temperature to prevent the premature precipitation of the solute.
The advantages of RESS are that it is a simple process, and relatively easy to implement on a small scale when a single nozzle is used. Another attractive characteristic of this process is its environmental benignity: it allows minimization of the use of organic solvent and the reuse the SCF in a continuous process. On the other hand, the main drawback, limiting the scaling of this process, is represented by the poor solubility of most pharmaceutical products in supercritical CO2. The CO2 is a non polar molecule with low molecular weight, scarcely able to dissolve drugs that, typically, are weak bases or acids and, therefore, show more or less pronounced polar characteristics. In the RESS technique, the solubility value, for obtaining a reasonable yield, should be in the order of 10-4 mole fraction. Otherwise, the low solubility can, in some instances, be overcome with appropriate tuning of the fluid density and/or using an adequate cosolvent. Cosolvents modify the polarity of the solvent phase in favour of the solute, thereby improving the solvent power. Enhancement factors values of 104-106 (defined as the measured solubility divided by the solubility in the SCF without cosolvent) are common, although even values as high as 1012 have been reported (Kompella and Koushik, 2001) Other limitations are poor predictive control of particle size and morphology along with the difficulty of scaling-up the process because of particle aggregation and nozzle blockage caused by cooling due to the rapid expansion of the supercritical solution (York, 1999).
RESOLV (Rapid Expansion of a Supercritical Solution into a Liquid Solvent)
The solution of the drug in liquid CO2 is prepared inside a high pressure syringe pump.
The solution is pumped into a heating unit to attain the desire temperature before the expansion through a laser-drilled orifice. The rapid expansion of the solution occurs into an aqueous medium at ambient pressure. Various water-soluble polymers could be added to the aqueous medium for stabilizing the nanoparticles suspension (Meziani et al., 2005).
1.2.2 Precipitation using supercritical fluids as antisolvent
Gallagher et al. (Gallagher et al., 1989) first proposed a SCF process alternative to RESS to overcome the limitation of poor solubility of most organic compounds in SC-CO2. This technique was first tested to micronize explosives because milling generates high local temperatures, while the use of CO2 as an antisolvent allowed to proceed at milder temperature. This method is based on the ability of a liquid to solubilize a large amounts of gaseous CO2. The antisolvent must show a low affinity for the solute but at least partial miscibility with the organic phase. The nucleation and the consequent growth of crystals from the solute/organic solvent/antisolvent system are governed by the diffusion of the antisolvent into the organic phase and the evaporation of the organic solvent into the antisolvent phase (Figure 6).
Figure 6. Single droplet (solvent + solute) as the smallest unit where the crystallization occurs. G gas (antisolvent), D diffusion of the antisolvent into the solution, E evaporation of the organic solvent into the
The volume expansion caused by the antisolvent diffusion lowers the solubility of the solute due to density reduction. On the other hand, the solvent evaporation into the gas
D solvent +
phase increases the solute concentration. The combined phenomena lead to supersaturation, nucleation and particle formation (Bristow et al., 2001).
Contributions from thermodynamics, fluid dynamics, and nucleation kinetics are necessary to describe the antisolvent precipitation. Mass transfer coefficient governs the rate of mutual transport of the SCF into the solvent phase and viceversa. The relationship that describes the rate of mutual transport for component (Ni) is represented by a simple solution of the Fick’s law,
Ni = KL,SC a (Cie – C) 
where, a is the mass transfer area, Cie is the saturated concentration in the respective supercritical (SC) or liquid (L) phase, C is the concentration in the bulk liquid or SC phase, and KL,SC is the overall mass transfer coefficient either in the liquid or SC phase (Bristow et al., 2001).
Since crystallization is the opposite of dissolution, the diffusion theory (Brunner, 1904, Nernst, 1904, Noyes and Whitney, 1897) can be applied. Therefore, equation 2 holds for the solute mass transfer rate (Nso) over the crystal surface area, ac :
Nso = Kso ac (Css – Cs) 
here, Css is the supersaturated concentration and Cs is the solubility (both in the liquid phase), and Kso is the solute mass transfer coefficient (Figure 7).
Figure 7. Scheme of the concentration profile at the crystal-supersaturated solution interface; Cs equilibrium concentration, Css supersaturated concentration, h thickness of the diffusional path lenght
To achieve a high supersaturation and thus particle formation level, the mass transfer rate has to be improved, by increasing the mass transfer area, the concentration gradient, or the SCF/solvent ratio.
As far as the surfacial mass transfer is concerned, it can be increased by spraying a phase into the other. In this case, the nucleation of the particle depends on the efficiency of the droplets generation. The distribution of the droplet size has to be as homogeneous as possible. The Weber number (Nwe), which is the ratio between disruptive fluid dynamic and inertial forces and the shape maintaining interfacial forces, determines the droplet size.
Nwe = σ ν ρA A2D
where ρA is the density of the antisolvent, v is the relative velocity, D is the jet diameter 2A and σ is the interfacial tension (Brunner, 1904). The higher the Weber number, the lower the droplet size and viceversa.
Another important factor that must be considered in an antisolvent process is the efficiency of the mixing between the SCF and the solution. The Reynolds number (NRe) describes the mixing efficiency
NRe = η ρvsL
where, ρ is the density of the fluid, υs is the mean fluid velocity, L is the characteristic length (equal to the diameter if the cross-section is circular), and η is the fluid viscosity. It is possible to obtain a complete mixing at a high Reynolds numbers (> 10,000) that lead to dry particles with little agglomeration. In this situation, the flow is dominated by inertial forces, producing random eddies, vortices and other flow fluctuations (turbulent flow). At low Reynolds numbers, the viscous forces prevail, and the flow is characterized by smooth, constant fluid motion (laminar flow) (Shekunov et al., 1999). The nozzle geometry, the nature of the solvent and of the SCF are the main factors influencing the parameters described above. However, it must be underlined that the density of the antisolvent, which is one of the more easily tunable parameter (via temperature and/or pressure variation) in a SCF, can be considered the key factor of the process.
Since the driving force for crystallization is the supersaturation, other operative parameters, such as solute concentration, solvent to SCF ratio influence the characteristics of the product (Werling and Debenedetti, 1999).
The antisolvent process is a batch discontinuous process; its main disadvantage is the difficulty to reach a complete removal of the residual solvent. The regulatory authorities clarified that the amount of residual solvent in the crystallized powder must not exceed predetermined concentrations (USP 30, 2007). For this reason, a final washing step of the precipitated particles with supercritical CO2 alone may be required to remove residual traces of organic solvents and to prevent condensation during depressurization.
Different experimental designs of antisolvent processes are known and can be classified on the basis of different mixing modes between the solution and the SCF.
GAS (Gaseous Anti Solvent)
GAS is a batch technique which entails the gradual introduction of CO2 inside a vessel filled with the solution of the solute of interest (Figure 8).
Figure 8. Schematic representation of GAS
The CO2 is pumped in from the bottom of the vessel, until the fixed pressure is reached.
The main advantage of this technique is that, by introducing the SCF through the bottom of the vessel, a good mixing of solvent and antisolvent can be reached.
PCA (Particles by Compressed Antisolvent), SAS (Supercritical Antisolvent), ASES (Aerosol Solvent Extraction System)
In these three arrangements CO2 (supercritical for SAS, or subcritical for PCA) is first pumped inside the high pressure vessel until the system reaches the fixed conditions (pressure and temperature) Subsequently, the organic solution is sprayed through a nozzle into the SCF bulk and the particles are collected on a filter at the bottom of the vessel (Figure 9). ASES represents a modification implying the simultaneously spraying of the solution and antisolvent.
Figure 9. Schematic representation of PCA, SAS and ASES
SEDS (Solution Enhanced Dispersion by Supercritical Fluids)
SEDS is a technique developed by Hanna and York (Hanna and York, 1995). By this process the drug solution and the supercritical fluid are introduced simultaneously into the particle formation vessel through the mixing chamber of a co-axial nozzle (Figure 10 and 11).
Figure 10. Schematic representation of SEDS (Byrappab et al., in press)
The geometry of the nozzle allows to work at high Reynolds numbers (good mixing) and at low Weber number (small droplet size) by increasing the velocity of the fluid. Moreover, the use of a mixing chamber favors a higher mixing surface area that leads to a increase of the mass transfer (rate of mutual transport Ni in eq. 1). The high mass transfer causes a fast nucleation rate and the production of particles of small size with little agglomeration (Palakodaty and York, 1999).
SEDS has been further developed to process water soluble compounds (e.g. peptides and proteins) by using a co-axial three-component nozzle (Figure 11). The organic solvent, the SCF, and the aqueous solution, as separate streams, are introduced by means of the nozzle inside the vessel. This arrangement helps in overcoming problems associated with limited solubility of water in supercritical CO2 (Moshashaee et al., 2003).
Figure 11. Schematic representation of coaxial two and three fluid nozzle
All these characteristics make SEDS a highly controlled, reproducible technique compared to other antisolvent-based SCF processes. Furthermore, SEDS process proved to be suitable for scaling up and manufacturing according to GMP requirements (York et al., 1998).
1.2.3 CO2 -Assisted Spray-Drying
These techniques are aerosolization based methods where the supercritical CO2 is used to assist the nebulization of the solution of the compound to be processed. The mechanism of the process is close to classic micronization by spray-drying: the SCF and the solution are intimately mixed and sprayed in a drying atmosphere. Claimed advantages of this process are: the minimal decomposition of thermally labile drugs, the absence of a high pressure vessel, and the small size of produced particles (below 3 µm in diameter) (Charbit et al., 2004).
CAN-BD (Carbon dioxide Assisted Nebulization with a Bubble Dryer®)
This process (Sievers and Karst, 2000) is particularly useful for substrates that are significantly soluble in water. Three steps are involved in the method. The drug is dissolved or suspended in water or alcohol (or both), and mixed intimately with near- critical or supercritical CO2 by pumping both fluids through a near zero volume tee to generate an emulsion. The carbon dioxide does not solubilize the compound, but it is soluble in water. The emulsion expands through a flow restrictor into a drying chamber at
atmospheric pressure to generate aerosols of microbubbles and microdroplets that are dried by a flux of warm nitrogen (Figure 12).
Figure 12. Schematic representation of CAN-BD
SAA (Supercritical Fluid-Assisted Atomization)
In this process (Reverchôn, 2002) supercritical CO2 and a solution (in water or organic solvent) are mixed and sprayed into a vessel loaded with stainless steel perforated saddles that assures a large contact surface between liquid solution and the SCF, at conditions near the atmospheric pressure under a flow of hot N2 (Figure 13).
Figure 13. Schematic representation of SAA
The main differences between CAN-BD and SAA processes are the region where the mixing is achieved and the extent of solubilization of SC-CO2 in the liquid solution where the solute is dissolved.
1.2.4 Precipitation from gas saturated solutions
These processes use the supercritical fluids to obtain a molten material or a ternary mixture solute-solvent-compressed gas that are depressurized by rapid reduction of the system to atmospheric pressure in an expansion chamber. PGSS is the method that exemplifies this group.
PGSS (Particle formation from Gas-Saturated Solutions)
In the PGSS, the compressed gas (super- or sub-critical) is dissolved into a solution of a solute or into a melted material. The gas-saturated solution presents a low viscosity due to an increase in free volume. Moreover, the interfacial tension between gas and the liquid phase is lowered as the surface tension of the gas in the supercritical state is near zero. The solution is then expanded over a nozzle from a supercritical status to ambient pressure. It causes a supersaturation of the gas and an intense expansion of the nucleated gas bubbles leading to explosion of the molten material into fine particles (Graser and Wickenhaeuser, 1982) (Figure 14).
Figure 14. Schematic representation of PGSS
The advantages of this technique are numerous. The pressure used is lower than that used with RESS, the required amount of gas is smaller, no additional solvent is necessary, so no residual solvent traces can be found in the final product, it can work in continuous mode, while the antisolvent technique required a wash-out step to remove the solvent traces.
Furthermore, because of the high solubility of the compressed gas, a good process yield can be obtained. An interesting case is represented by the use of the PGSS technique to process the polymers. It is well known that compressed CO2 can act as a plasticizer and can decrease the melting point and/or glass transition of some polymers, (Kazarian, 2000, Kazarian et al., 2002, Pasquali et al., in press-c) so in this case, it is possible to use PGSS to load active substances on this melted polymer that form composite microspheres after decompression. The concept is simple and the substances both polymer and drug do not have to be soluble in the CO2. The main drawbacks of this technique are the poor control of the particle size that can, in some cases, leads to a broad particle size distribution, moreover the high temperature that can be required to melt some polymers may damage thermolabile compounds. Anyway, the balance between advantages and drawbacks is positive, and the technique is promising, several plants are running with capacities of some hundred kilograms per hour (Natex, Austria, Thar Technologies, USA, Uhde HPT, Germany).
DELOS (Depressurization of an Expanded Liquid Organic Solution)
In the DELOS technique, the compressed gas acts as a cosolvent. In fact the CO2 expands in an autoclave where a organic solution of the solute that has to be micronized is dissolved.
Then the ternary mixture solute-solvent-compressed gas is depressurized by rapid reduction of the system pressure to atmospheric pressure in an expansion chamber (Ventosa et al., 2001, Ventosa et al., 2003) (Figura 15).
Figure 15. Scheme of the equipment used for DELOS experiments. P: pump; S: heat exchanger; V: valve; F:
filter; R: high-pressure vessel; RC: recycling collector.
CPCSP (Continuous Powder Coating Spraying Process)
The CPCSP was proposed by Weidner et al., as an alternative technique for powder coating based on the PGSS (Weidner et al., 2001). In the CPCSP, the main components (binder and hardner) are melted in separated vessels to avoid a premature reaction of the polymers. The molten polymer are fed to a static mixer, here, the melts are homogenised with compressed carbon dioxide under pressure up to 220 bar. In the static mixtures, the three flows are not only intensively mixed, but a part of compressed gas dissolves in the polymer mixture. Then, the solution formed in the mixer expands via a nozzle to a spray tower.
A qualitative technological assessment of the different supercritical fluids based techniques is reported in the table 3.
Table 3. Technological features of different supercritical fluids based techniques
RESS GAS/SAS/PCA PGSS
Process Discontinuous Semicontinuous Continuous Gas demand High Medium Low Pressure High Low to medium Low to medium Solvent None Yes None Volume of pressurized Large Medium to large Small equipment
Separation gas/solid Difficult Easy Easy Separation gas/solvent Not required Difficult Not required
1.3 Phase behaviour
When supercritical fluids based processes are used, it is important to take into account both the solid-fluid phase behaviour (solubility) and liquid-fluid phase behaviour (miscibility) to understand and be able to govern the process.
For a full understanding of the phase equilibria for mixtures, it is important to consider the geometric constraints on their topology imposed by the phase rule:
f = c-p+2 
where f is the degree of freedom, c the number of components, and p the number of phases.
This equation (Gibbs’s phases rule) provides the number of independent variables that must be set in a equilibrium system. For example, for a two-phase binary mixture the regions of the equilibrium of the phases can be obtained either by experiment or calculation if the temperature and pressure are fixed. In a two-phase ternary mixture, one more variable, usually the overall mixture composition, must also be fixed.
1.3.1 Unitary system (one component)
A substance can exists in three different states: solid, liquid and gas depending on the two variables temperature (T) and pressure (p), as shown in Figure 3.
Equilibrium between different phases is along the saturation curves and the three phases co-exist in equilibrium at the triple point. The evaporation curve (equilibrium between liquid and vapour phases) ends at the critical point.
1.3.2 Binary system (two components)
In the case of the binary system, the phase boundary can be represented on a T-x (temperature plotted against the mole fraction of the mixture at a constant pressure) or P-x diagram (pressure plotted against the mole fraction of the mixture at a constant temperature), then the locus of the critical points are represented on a P-T space.
In Figure 16 a P-x diagram of CO2 and ethanol at 70 °C is reported. The phase diagram was calculated using the PE-2000 software developed by the Technische Universität Hamburg-Harburg (Germany). The program was developed to model phase equilibria with a variety of equations of state. In particular for this diagram, the binary systems was calculated with the Peng-Robinson Equation of State (PR-EOS) using quadratic mixing rules. The binary interaction coefficients (kij) and critical parameters (Tc, pc, ω) for the pure components are taken from the literature.
CO2 mole fraction
0.0 0.2 0.4 0.6 0.8 1.0
0 20 40 60 80 100 120
Figure 16. P-x diagram of ethanol and CO2 at 70 °C xc
At low pressures the mixture only shows a homogeneous vapour phase. With pressure increase the mixture exhibits a dew point (at this point the liquid phase shrunk to an infinitely small droplet which is in equilibrium with a vapour phase). With a further pressure increase, a region where both the liquid and gas phase are present is reached. The composition of the vapour and liquid phase can be obtained by the length of the tieline (virtual connections between co-existing phases). The increase of the pressure leads, contrary to the case of a pure component system, not only to a volume change, but also system composition. At the composition lower than xc, with a further pressure increase, the mixture crosses first the bubble point curve (at the bubble point the vapour phase shrunk to an infinitely small bubble which is in equilibrium with a liquid phase) and then it reaches a single homogeneous liquid phase. At the composition xc the mixturedoes not cross the bubble point, but it reaches the critical point. Above Pc at that temperature (70 °C) all mixtures are supercritical (homogeneous region where ethanol and CO2 are completely miscible). Note that the critical point in a binary mixture is always at the maximum of the bimodal curve. Furthermore, the critical point is the point where dew and bubble curve meet; therefore the critical point is a dew and a bubble point at the same time. At compositions higher then xc the mixtures crosses the dew point curve twice with increasing pressure. It appears that the mixture is vaporizing again with increasing pressure. This phenomenon is called retrograde condensation.
Another way to plot the binary phase equilibria is a T-x diagram. In this case, the change in temperature are plotted against the composition at a constant pressure. The resulting diagrams are usually very similar to the corresponding P-x diagrams, but appear to be upside down.
A third way to represent fluid phase equilibria is the P-T diagram at constant composition.
Van Konynenberg and Scott (van Konynenburg and Scott, 1980) had grouped the possible phase diagrams of liquid-fluid phase behaviour in five major schematic classes which are represented in Figure 17.
Figure 17. Phase Behaviour Classification for Binary Mixtures according to Van Konynenburg and Scott
The simplest binary mixture is the Type 1. The dark lines represent the vapour-liquid line of the pure components that terminate in the critical point (C1 and C2), while the critical curve runs continuously from the critical point of the more volatile component (C1) to that of the less volatile component (C2). Above the critical line the fluids are completely miscible. Type II behaviour is similar to Type I with an additional liquid-liquid critical line that commences at low temperatures rising steeply to high pressures from an Upper Critical End Point (UCEP). At this point, the liquid and gaseous phases of one component become identical critical in the presence of the liquid phase of the second component (liquid-liquid-vapour three-phase line). This indicates that, at low temperature, an immiscibility region between fluid and liquid is present.
Type V fluid phase behaviour is characterised by two critical lines. The critical line from the component with the lower critical temperature terminates in an Upper Critical End Point (UCEP) whereas the other critical line ends in a Lower Critical End Point (LCEP).
At temperatures between LCEP and UCEP three phases co-exist (liquid 1 + liquid 2 + vapour), but above the UCEP the fluids become completely miscible mimicking Type I behaviour, although with significantly higher mixture critical pressures than Type I systems.
The difference between Type IV and Type V is identical to Type I and Type II. In Type IV a liquid-liquid critical line commences at low temperatures from an Upper Critical End
Point (UCEP) and rises steeply to high pressures, leading to similar operating restrictions as Type II.
In Type III phase behaviour, the vapour-liquid critical line commencing from the critical point of the component with the higher critical temperature only extends partly to the critical point of the other component before rising to high pressures. Furthermore, this critical locus displays a continuous transition between vapour-liquid and liquid-liquid equilibrium. The vapour-liquid line commencing from the critical point of the component with the lower critical temperature ends again in an UCEP. Fluids that show this kind of phase behaviour are completely immiscible with solvents.
The P-T projection are useful for a rationale design of those processes that use the SCF as antisolvent. Potential antisolvents can be classified into three categories according to their phase behaviour with solvents:
• Category I (Type I or Type II fluid phase behaviour)
CO2, N2O, CHF3, CH2F2, HFAs, CnH2n (4<n<12), CnH2+n (4<n<12), etc.
• Category II (Type V or Type IV fluid phase behaviour) CnH2n (1<n<5), CnH2+n (1<n<5), Xe, etc.
• Category III (Type III fluid phase behaviour) He, Ar, N2, H2, CO, SF6, CH4, etc.
Fluids belonging to category I do not introduce limitations to the process, and are probably the least potent antisolvents. Fluids of category II are non-polar and therefore good antisolvent for solids. However they have the restriction on the antisolvent process of a limited range of operating temperature and pressure. Fluids of category III are immiscible with solvents and therefore are also good antisolvent for solids, but the immiscibility creates processing problems that might be difficult to overcome (The solvent can not to be extracted from the processed material).
It has to be remembered that it is possible to represent the whole P-T-x space in three dimensional diagram. But, usually binary phase diagrams are not represented in this way for two reasons: normally there are not enough data available to support the graph, and these diagrams tend to be very complicated. Anyway, it is possible to derive P-x and T-x projections of the mixture from the P-T diagram.
As stated before, unlike gases at low pressure, supercritical fluids show a remarkable solvent power for the solids. As an example, Figure 18 shows the solubility changes of nifedipine in supercritical carbon dioxide as function of the pressure (Knez et al., 1995).
The solubility decreases with increasing temperatures up to pressures below the cross over region, which is about 220 bar for this system, and then increases. This is explained taking into account two different aspects: an increase of the temperature leads to a increase of molecular mobility and so at higher solubility, but on the other hand, an increase in temperature decreases the CO2 density and therefore its solvent power. At low pressure a decreasing of the solubility with the increase of temperature, due to the density change, is observed, while above the cross over pressure the kinetic aspects become more important.
Figure 18. Solubility of nifedipine in the supercritical CO2 (Knez et al., 1995)
A schematic diagram for a SCF and solid system is represented in Figure 19, where the P- T diagram is reported with the P-x sections at three different temperatures.
Figure 19. Representative diagram for a SCF+solid system
The diagram generalizes the phase behaviour for systems in which the melting point of the solid is significantly higher then the critical temperature of the fluids. This diagram represents a system where the solid and the SFC are very dissimilar in molecular size, polarity, structure etc, namely when the SFC is not very soluble in the molten solute.
The critical curve shows two branches. One branch runs in the P-T projection from the critical point of the more volatile component to a point of intersection with a three-phase curve S2LG which is called Lower Critical End Point (LCEP). The second branch of the critical curve runs from a point of intersection with a second branch of the S2LG (Upper Critical End Point, UCEP) and the critical point of the less volatile component. The three phase line S2LG starts in the triple point of the pure less volatile component. From the same point commences also a line that rises steeply to high pressures; this represents the liquid-solid line of the pure component.
In the same Figure also a P-x sections at three different temperature are reported. At temperature TA, above the critical temperature of the more volatile component and below the temperature of the LCEP, a two phase region S2G is separated from a S2L region, a homogeneous liquid region and a LG region by three-phase equilibrium S2LG.
Furthermore the LG region ends at high pressure in a L=G critical point.
At temperature TB the LG region disappears and the S2G region and S2L region merge into one solid-fluid two phases region, which exhibits a horizontal tangent at the UCEP. This results in a sharp increase of the solubility of the solid in SCF.
For the temperature TC between the UCEP and the triple point of the less volatile component, the P-x projection is given in the same Figure.
As underlined before, for this type of binary mixtures, the melting point of the solid is higher than the critical temperature of the SCF. Sometimes, in the presence of SCF, the melting point of the solid decreases with the increase of pressure. The reason of this depression is that, as the pressure increases, more and more as the gas dissolves into the solid (usually polymers) decreasing its melting point. In this case the phase diagram changes in shape and the right side branch of the diagram becomes close to the branch referred to the SCF critical line (Figure 20 a,b,c). In Figure 20 a, it is possible to note that the three phase curve L2L1G ends at low temperature in a quadruple point SL2L1G where four phases coexist. In the quadruple point three other three-phase curves terminate. The SL2L1 curve runs steeply to high pressure and ends in the UCEP where this curve intersects the critical curve. The SL2G curve runs to the triple point of the less volatile pure component and the SL1G curve runs to lower temperature. When the melting point of the less volatile component increases (e.g. in the case of the polymer with higher molecular weight) the melting curve of the solid shifts to higher temperature; and also the quadruple point shifts to higher temperature (b) and eventually coincides with the LCEP of the more volatile component (c).
Figure 20. P-T diagrams for SCF+solid system when the SFC decreases the melting point of the solid
1.3.3 Ternary system (three components)
A two phase ternary system has three degrees of freedom and it is usually represented in so-called Gibbs-triangles, where compositions is plotted at constant pressure and temperature.
A typical three component system of CO2-methanol-water is drawn in Figure 21.
Figure 21. Gibbs-triangle for an arbitrary ternary mixture
The corners of a Gibbs-triangles represent the pure components, the edges the three binary systems (H2O-CO2, CO2-CH3OH, CH3OH-H2O), so any ternary mixture lies inside the borders of the triangle. The binodal curve (defined as the line which envelopes the region where liquid and vapour phases are present) is large indicating a large region of the immiscibility in this ternary system. The bottom of the triangle represents the binary system CO2-H2O, it is possible to see that only a small amount of either component is miscible with the other, while CH3OH and water and CH3OH and CO2 are miscible in all proportions. The tielines inside the binodal curve are not parallel to each other as for the binary system (Figure 16), and consequently, the critical point does not lie at any extreme point. Anyway, also in this case, the critical point is the point where dew and bubble curves meet each other, here, at fixed temperature, pressure and composition the three fluids are completely miscible. The non-parallelity of the tielines offers good possibility for the antisolvent process because only changing the flow ratios of the three fluid components, and without changing temperature and pressure it is possible to influence the obtained product.
1.4 Polymers processing using SC-CO2
SC-CO2 is used in the area of polymer processing such as polymer modification, blending, foaming, and formation of polymer composites due to its unique properties. CO2 is able to plasticize many polymers owing to its capability to solubilize into them. This property causes an increase of chain mobility resulting in a decrease either of the glass transition temperature, in the case of amorphous polymers, or of melting point, in the case of semicrystalline polymers. Both in the rubbery or in the liquid state the polymer can be easily manipulated.
A peculiar characteristic is that CO2 is a “temporary” plasticizer, CO2 is a gas under standard conditions so it is easily removed from the final product at the end of the process.
Furthermore, for the intrinsic properties of the CO2, the processing of polymeric material is possible at mild operative conditions and the enhancement of the solute diffusion is possible by changing the process parameters.
1.4.1 Polymer-CO2 phase behaviour (Liquid-Liquid phase behaviour)
In Figure 22, the T-x, phase diagrams typical of an amorphous and monodisperse polymer- CO2 system at three different pressure are reported.
Figure 22. T-x phase diagram typical of an amorphous and monodisperse polymer-CO2 system T
polymer concentration UCST P1
T LCST UCST
The T-x sections of the L-L phase equilibria indicate the miscibility region of the polymer- CO2 system, and, on the basis of different pressure, they may show upper critical, lower critical or hourglass-type demixing behaviour.
In particular, at elevated pressure (P1) the section shows a LL miscibility gap in continuous with a maximum that represents the upper critical solution temperature (UCST);
at intermediate pressure (P2) the miscibility gap becomes discontinuous with a maximum at UCST and a minimum called lower critical solution temperature (LCST); at pressure lower than critical pressure (P3) the miscibility gap becomes an hourglass-shaped without the critical point. The absence of the critical point underlines that in this case the system is immiscible at all temperatures within a limited concentration range (Folie and Radosz, 1995).
It has to be underlined that the reported diagrams are idealised, because, in the real system, the curve is highly asymmetric with the maximum shifted toward the CO2-rich phase.
Furthermore, for the polydispersity of polymers, the UCST does not coincide with the maximum of the phase boundary, but it is shifted to higher polymer concentrations (Folie and Radosz, 1995).
1.4.2 Pressure Induced Phase Separation (PIPS)
In polymer processes based on SCF such as blending, formation of polymer composites without the use of organic solvents, extrusion, etc., the concentration of CO2 into the polymer might be kept below the saturation limit to avoid the phase separation and to work in a homogeneous phase. (Nalawade et al., 2006a). If the homogeneous polymer solution is necessary condition for the process, the pressure reduction is an integral step in the recovery of the end product; for this reason, there is a great interest in the study of how a homogeneous polymer solution may undergo phase separation as a result of a change in pressure (Zhuang and Kiran, 1998).
In Figure 23, a more detailed schematic representation of the L-L phase behaviour is reported to explain the phenomenon of PIPS.
Figure 23. Schematic representation of pressure-induced phase separation in the pressure-composition phase diagram at fixed temperature, modified from (Palakodaty and York, 1999)
The phase diagram shows the binodal curve which, as stated before, is defined as the line which divides the stable one phase region from the region in which two phase coexists in equilibrium, and the spinodal curve, which divides the two phases region into metastable and unstable portions. The region between the spinodal and binodal curves is the metastable region.
If the system is at pressure higher than P1, is in a stable one phase region (above the critical point of the mixture), then, by decreasing the pressure, the system goes into two phases region at a pressure P2. As indicated in Figure 23, three different pressure reduction paths are possible (AB, EF, CD) for solutions at three different polymer concentrations, all starting at an initial pressure P1 and ending at a final pressure P2. The reduction in pressure creates a new phase formation that proceeds in two different paths (AB=CD) and leads to a different microscopic separation mechanism: i) nucleation and growth mechanism in the case of paths AB and CD (when metastable regions are entered) and ii) spinodal decomposition mechanism in the case of EF path (the unstable region is entered).
In the case of nucleation and growth mechanism, the system is brought into the metastable region and so energy-intensive demixing occurs, consequently, the nuclei of the new phase form and grow into dispersed droplets in a continuous polymer-rich phase.
In the case of the spinodal decomposition mechanism, the system is brought into thermodynamically unstable region and the system demixes spontaneously, forming two cocontinuous phases.
The spinodal decomposition mechanism can occur also in the case of paths AB and CD when the pressure is rapidly decrease and therefore, the system goes quickly in the unstable region.
The different mechanisms of the phase separation, as well as the kinetic are very important parameters because they can lead to final product with different morphologies, ranging from powders, to porous structures of different size and distributions (Zhuang and Kiran, 1998).
Interesting experimental works about the kinetics of PIPS in solutions of polymer and gas at high pressure using time- and angle-resolved light scattering were carried out by Kiran and co-workers (Liu and Kiran, 1999, Xiong and Kiran, 2000, Zhuang and Kiran, 1998).
1.4.3 Solubility of CO2 in polymers and viceversa
The solubility data of CO2 into polymer and polymer in SC-CO2 at various temperatures and pressures provide a very useful criteria to determine the operative conditions for all type of polymer processing.
The solubility of CO2 is largely based on its ability to weakly interact with functional groups present along the molecular chains of the polymers. The CO2 molecule can be seen as a weak Lewis acid that can interact with the basic sites of the polymer; this can be considered the main contributor to its solubility. The evidence of this interaction was obtained spectroscopically by studying interactions between CO2 and polymers containing basic functional groups (carbonyl group or phenyl rings) (Kazarian et al., 1996).
In the last decade, many experimental methods have been applied to investigate the solubility of CO2 in polymers at elevated pressure. The most commonly used are: phase separation method, pressure decay method, gravimetric method, chromatographic method and spectroscopic method.
In the phase separation method, a molten polymer is exposed to the CO2 at desired pressure in an autoclave. After reaching the polymer/CO2 equilibrium system (typically few hours), samples are taken from the two phases: a polymer-rich and a CO2-rich phase.
The amount of CO2 in the polymer-rich phase is determined with a flowmeter (Weidner et al., 1997), or by measuring the volume of CO2 corresponding to the displacement of water level in an inverted graduated tube which is immersed in CO2 saturated water (Daneshvar